Gregory Harry LIGO Scientiﬁc Collaboration, American University, 4400 Massachusetts Ave NW, Washington DC 20016 [email protected]
Steve Penn LIGO Scientiﬁc Collaboration, Hobart and William Smith Colleges, 126 Eaton Hall, Geneva NY 14456 [email protected]
Garrett Cole Crystalline Mirror Solutions, 114 E. Haley Street, Santa Barbara CA 93101 [email protected]
GariLynn Billingsley LIGO Laboratory, California Institute of Technology, 1200 E. California Blvd., Pasadena CA 91125 billingsley [email protected]
Matthew Evans LIGO Laboratory, Massachusetts Institute of Technology, 185 Albany Street, Cambridge MA 02139 [email protected]
Geoffrey Lovelace LIGO Scientiﬁc Collaboration, California State University Fullerton, 800 N. State College Blvd., Fullerton CA 92834 [email protected]
Kieran Craig LIGO Scientiﬁc Collaboration, Physics and Astronomy, University of Glasgow, Glasgow UK G12 8QQ [email protected]
Abstract: Substrate-transferred single-crystal semiconductor heterostructures are effective as low-thermal-noise optical coatings for small beams. We discuss developing GaAs/AlGaAs coatings at a size scale relevant to interferometric gravitational wave detectors such as LIGO. © 2018 Optical Society of America OCIS codes: 310.1620, 270.2500, 350.1270
1. Introduction, Background, and Requirements Gravitational wave detectors like LIGO  and Virgo  are optical instruments designed to detect waves predicted in Einstein’s General Theory of Relativity. They have had recent success by detecting gravitational waves from black hole and neutron star systems [3–5]. When these detectors reach their design sensitivity  around 2021, they will be limited by thermal noise  from the mirror coatings on the test masses . Thermal noise is the random motion of atoms and is determined by temperature, material Young’s moduli, beam size of the readout laser, and the mechanical loss of the coating, the ratio of the imaginary to the real part of the Young’s modulus. Most of these quantities are known for coating materials or easily determined. The exception is mechanical loss, which must be measured. Substrate-transferred single-crystal aluminum gallium arsenide/gallium arseninde (AlxGa1 xAs/GaAs) (AlGaAs) multilayer Bragg stacks have proved effective as optical coatings for precision measurement applications . AlGaAs coatings are grown on gallium arsenide wafers using molecular beam epitaxy. They then can be moved to substrates of various materials including fused silica glass where they adhere without use of intermediate materials. As an inter- ference coating, the reﬂectivity can be modiﬁed by changing the layer count, the individual layer thicknesses and in this system speciﬁcally, by adjusting aluminum content in the low refractive index AlGaAs layers. The Advanced LIGO test masses are 40 kg optics made from fused silica, 34 cm diameter and 20 cm thick. These optics have an ion beam sputtered coating of titania-doped tantala  and silica. Future interferometeric gravitational wave detectors with increased sensitivity to see further into the universe require lower coating thermal noise.
2. Measurements, Modeling, and Future Plans Direct measurements of thermal noise from AlGaAs mirrors have been made in the quantum measurement commu- nity [8, 9]. The beam size in these experiments is typically tens of microns to one millimeter, which increases the thermal noise and makes it possible to measure in a laboratory setting. Thermal noise consistent with more than a factor of two improvement over current LIGO mirror materials has been observed in these experiments. Conﬁrmation of this result within the gravitational wave detection community is in progress. The mechanical quality factor of silica disks coated with AlGaAs have been measured to determine mechanical loss. These have been reported as a single value, although the samples are alternating layers of GaAs and AlGaAs and each material separately has multiple loss angles. Initial measurements yielded loss angles of f 5 10 4. Improvements ⇡ ⇥ to coating uniformity and to the coating transfer process for coatings sizes up to 75 mm in diameter, have lowered ⇠ the loss angle to 2 10 5, which is comparable to the best loss observed in direct thermal noise measurements . ⇠ ⇥ AlGaAs is a crystal with three independent loss angles. Each of these loss angles serves as a source of thermal noise. The full implications of these mutliple loss angle for both interpretation of Q measurements and prediction of thermal noise is being analyzed. An open source computational tool that numerically solves the elastic problem to predict Brownian thermal noise from crystalline coatings has been developed. This code has successfully reproduced known results on amorphuous coatings and correctly scales with beam size, coating thickness, and coating diameter. The principle engineering challenge to use of AlGaAs coating on gravitational wave detectors is the size. The largest AlGAs coating to date is 20 centimeter diameter, while more than 30 centimeters is needed, with excellent optical and mechanical properties across the whole diameter. Samples for optical tests at the LIGO Laboratory at Caltech are being prepared for measurement the summer of 2018. Samples suitable for mechanical loss measurements will also be prepared from the same deposition run to measure Q on low defect AlGaAs. Q samples with just AlGaAs and GaAs will also be measured for mechanical loss, to determine how much each individual material contributes to thermal noise. Modeling and theory efforts on the full crystalline nature of AlGaAs’s stiffness matrix continue as well.
References 1. B. P. Abbott et al. (The LIGO Scientiﬁc and Virgo Collaborations), ‘’GW150914: The Advanced LIGO De- tectors in the Era of First Discoveries”, Physical Review Letters 116, 131103 (2016). 2. F. Acernese et al. (Virgo Collaboration), ‘’Advanced Virgo: a second-generation interferometric gravitational wave detector”, Classical and Quantum Gravity 32, 024001 (2015). 3. B. P. Abbott et al. (The LIGO Scientiﬁc and Virgo Collaboratiosn), ‘’Observation of Gravitational Waves from a Binary Black Hole Merger”, Physical Review Letters 116, 061102 (2016). 4. B. P. Abbott et al. (The LIGO Scientiﬁc and Virgo Collaborations), “GW170814: A Three-Detector Observation of Gravitational Waves from a Binary Black Hole Coalescence”, Physical Review Letters 119, 141101 (2017). 5. B. P. Abbott et al. (The LIGO Scientiﬁc and Virgo Collaborations), “GW170817: Observation of Gravitational Waves from a Binary Neutron Star Inspiral”, Physical Review Letters 119, 161101 (2017). 6. The LIGO Scientiﬁc Collaboration, ‘’Advanced LIGO: the next generation of gravitational wave detectors”, Classical and Quantum Gravity 27, 084006 (2010). 7. P. R. Saulson, ‘’Thermal noise in mechanical experiments”, Physical Review D 42, 2437 (1990). 8. “Optical Coatings and Thermal Noise in Precision Measurements”, ed. G. M. Harry, T. P. Bodiya, R. DeSalvo, Cambridge University Press (2012). 9. G. D. Cole, W. Zhang, M. J. martin, J. Ye, and M. Aspelmeyer, ‘’Tenfold reduction of Brownian noise in high-reﬂectivity optical coatings”, Nature Photonics 7, 644 (2013). 10. G. M. Harry et al., ‘’Titania-doped tantala/silica coatings for gravitational-wave detection”, Classical and Quan- tum Gravity 24, 405 (2007).